#------------------------------------------------------------------------------
#$Date: 2017-02-07 17:13:06 +0200 (Tue, 07 Feb 2017) $
#$Revision: 191892 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/10/35/2103537.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2103537
loop_
_publ_author_name
'Pavlovska, A.'
'Werner, S.'
'Maximov, B.'
'Mill, B.'
_publ_section_title
;
 Pressure-induced phase transitions of piezoelectric single crystals
 from the langasite family: La₃Nb~0.5~Ga~5.5~O₁₄ and
 La₃Ta~0.5~Ga~5.5~O₁₄
;
_journal_issue                   6
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              939
_journal_page_last               947
_journal_paper_doi               10.1107/S0108768102010273
_journal_volume                  58
_journal_year                    2002
_chemical_formula_sum            'Ga5.54 La3 O14 Ta0.46'
_chemical_formula_weight         1110.22
_chemical_name_systematic        ?
_space_group_IT_number           150
_symmetry_space_group_name_Hall  'P 3 2"'
_symmetry_space_group_name_H-M   'P 3 2 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   8.089
_cell_length_b                   8.089
_cell_length_c                   5.064
_cell_measurement_temperature    293(2)
_cell_volume                     287.0
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_pressure         6.64E+6
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.599
_diffrn_measured_fraction_theta_max 0.599
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0696
_diffrn_reflns_av_sigmaI/netI    0.0425
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       4
_diffrn_reflns_limit_l_min       -4
_diffrn_reflns_number            1685
_diffrn_reflns_theta_full        31.98
_diffrn_reflns_theta_max         31.98
_diffrn_reflns_theta_min         2.91
_exptl_absorpt_coefficient_mu    28.132
_exptl_crystal_density_diffrn    6.424
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             488
_refine_diff_density_max         1.702
_refine_diff_density_min         -1.411
_refine_diff_density_rms         0.423
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   -0.08(5)
_refine_ls_extinction_coef       0.153(14)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.016
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     28
_refine_ls_number_reflns         427
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.016
_refine_ls_R_factor_all          0.0398
_refine_ls_R_factor_gt           0.0391
_refine_ls_shift/su_max          0.763
_refine_ls_shift/su_mean         0.027
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1000P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1060
_refine_ls_wR_factor_ref         0.1075
_reflns_number_gt                424
_reflns_number_total             427
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            sn0021-6.64cad4.cif
_cod_data_source_block           6.64cad4
_cod_depositor_comments
;
The _diffrn_ambient_pressure was taken from the original data block
header, after comparison with the paper text and supplementary
material.

Saulius Gra\<zulis
;
_cod_database_code               2103537
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'y, x, -z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -x+y, -z'
'x-y, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
La La -0.42909(11) 0.0000 0.0000 0.0142(4) Uani 1 2 d S
Ga1 Ga 0.0000 0.0000 0.0000 0.0145(6) Uani 0.50 6 d SP
Ta Ta 0.0000 0.0000 0.0000 0.0145(6) Uani 0.50 6 d SP
Ga2 Ga -0.6667 -0.3333 0.4706(7) 0.0127(7) Uani 1 3 d S
Ga3 Ga -0.7650(2) 0.0000 -0.5000 0.0156(6) Uani 1 2 d S
O1 O -0.3333 0.3333 0.168(4) 0.019(3) Uiso 1 3 d S
O2 O -0.4562(15) -0.3047(16) 0.296(3) 0.026(2) Uiso 1 1 d .
O3 O -0.2207(14) -0.0734(15) -0.244(2) 0.020(2) Uiso 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
La La -0.2871 2.4523 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ta Ta -0.7052 6.5227 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ga Ga 0.2307 1.6083 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 La O3 68.1(5) 6 .
O3 La O2 107.7(4) 6 3_455
O3 La O2 139.5(4) . 3_455
O3 La O2 139.5(4) 6 5_455
O3 La O2 107.7(4) . 5_455
O2 La O2 100.1(6) 3_455 5_455
O3 La O1 123.7(3) 6 2_455
O3 La O1 79.5(3) . 2_455
O2 La O1 70.1(5) 3_455 2_455
O2 La O1 93.0(4) 5_455 2_455
O3 La O1 79.5(3) 6 .
O3 La O1 123.7(3) . .
O2 La O1 93.0(4) 3_455 .
O2 La O1 70.1(5) 5_455 .
O1 La O1 154.01(9) 2_455 .
O3 La O2 65.6(4) 6 .
O3 La O2 79.2(4) . .
O2 La O2 63.9(5) 3_455 .
O2 La O2 154.88(18) 5_455 .
O1 La O2 64.0(5) 2_455 .
O1 La O2 126.9(5) . .
O3 La O2 79.2(4) 6 6
O3 La O2 65.6(4) . 6
O2 La O2 154.88(18) 3_455 6
O2 La O2 63.9(5) 5_455 6
O1 La O2 126.9(5) 2_455 6
O1 La O2 64.0(5) . 6
O2 La O2 137.6(4) . 6
O3 La Ga2 85.7(3) 6 .
O3 La Ga2 110.8(3) . .
O2 La Ga2 31.3(3) 3_455 .
O2 La Ga2 129.6(3) 5_455 .
O1 La Ga2 64.2(5) 2_455 .
O1 La Ga2 111.0(4) . .
O2 La Ga2 32.6(2) . .
O2 La Ga2 164.7(3) 6 .
O3 La Ga2 110.8(3) 6 2_565
O3 La Ga2 85.7(3) . 2_565
O2 La Ga2 129.6(3) 3_455 2_565
O2 La Ga2 31.3(3) 5_455 2_565
O1 La Ga2 111.0(4) 2_455 2_565
O1 La Ga2 64.2(5) . 2_565
O2 La Ga2 164.7(3) . 2_565
O2 La Ga2 32.6(2) 6 2_565
Ga2 La Ga2 160.49(3) . 2_565
O3 La Ga1 34.0(3) 6 .
O3 La Ga1 34.0(3) . .
O2 La Ga1 130.0(3) 3_455 .
O2 La Ga1 130.0(3) 5_455 .
O1 La Ga1 102.99(4) 2_455 .
O1 La Ga1 103.00(4) . .
O2 La Ga1 68.8(2) . .
O2 La Ga1 68.8(2) 6 .
Ga2 La Ga1 99.754(17) . .
Ga2 La Ga1 99.755(17) 2_565 .
O3 La Ta 34.0(3) 6 .
O3 La Ta 34.0(3) . .
O2 La Ta 130.0(3) 3_455 .
O2 La Ta 130.0(3) 5_455 .
O1 La Ta 102.99(4) 2_455 .
O1 La Ta 103.00(4) . .
O2 La Ta 68.8(2) . .
O2 La Ta 68.8(2) 6 .
Ga2 La Ta 99.754(17) . .
Ga2 La Ta 99.755(17) 2_565 .
Ga1 La Ta 0.0 . .
O3 Ga1 O3 83.9(6) 2 3
O3 Ga1 O3 107.1(6) 2 .
O3 Ga1 O3 85.9(4) 3 .
O3 Ga1 O3 85.9(4) 2 6
O3 Ga1 O3 162.8(6) 3 6
O3 Ga1 O3 83.9(6) . 6
O3 Ga1 O3 85.9(4) 2 5
O3 Ga1 O3 107.1(6) 3 5
O3 Ga1 O3 162.8(6) . 5
O3 Ga1 O3 85.9(4) 6 5
O3 Ga1 O3 162.8(6) 2 4
O3 Ga1 O3 85.9(4) 3 4
O3 Ga1 O3 85.9(4) . 4
O3 Ga1 O3 107.1(6) 6 4
O3 Ga1 O3 83.9(6) 5 4
O3 Ga1 La 42.0(3) 2 2
O3 Ga1 La 42.0(3) 3 2
O3 Ga1 La 98.6(3) . 2
O3 Ga1 La 126.5(3) 6 2
O3 Ga1 La 98.6(3) 5 2
O3 Ga1 La 126.5(3) 4 2
O3 Ga1 La 98.6(3) 2 .
O3 Ga1 La 126.5(3) 3 .
O3 Ga1 La 42.0(3) . .
O3 Ga1 La 42.0(3) 6 .
O3 Ga1 La 126.5(3) 5 .
O3 Ga1 La 98.6(3) 4 .
La Ga1 La 120.0 2 .
O3 Ga1 La 126.5(3) 2 4
O3 Ga1 La 98.6(3) 3 4
O3 Ga1 La 126.5(3) . 4
O3 Ga1 La 98.6(3) 6 4
O3 Ga1 La 42.0(3) 5 4
O3 Ga1 La 42.0(3) 4 4
La Ga1 La 120.0 2 4
La Ga1 La 120.0 . 4
O3 Ta O3 83.9(6) 2 3
O3 Ta O3 107.1(6) 2 .
O3 Ta O3 85.9(4) 3 .
O3 Ta O3 85.9(4) 2 6
O3 Ta O3 162.8(6) 3 6
O3 Ta O3 83.9(6) . 6
O3 Ta O3 85.9(4) 2 5
O3 Ta O3 107.1(6) 3 5
O3 Ta O3 162.8(6) . 5
O3 Ta O3 85.9(4) 6 5
O3 Ta O3 162.8(6) 2 4
O3 Ta O3 85.9(4) 3 4
O3 Ta O3 85.9(4) . 4
O3 Ta O3 107.1(6) 6 4
O3 Ta O3 83.9(6) 5 4
O3 Ta Ga3 97.9(3) 2 4_445
O3 Ta Ga3 54.3(3) 3 4_445
O3 Ta Ga3 31.7(3) . 4_445
O3 Ta Ga3 113.8(3) 6 4_445
O3 Ta Ga3 160.1(3) 5 4_445
O3 Ta Ga3 87.3(3) 4 4_445
O3 Ta Ga3 31.7(3) 2 4_446
O3 Ta Ga3 113.8(3) 3 4_446
O3 Ta Ga3 97.9(3) . 4_446
O3 Ta Ga3 54.3(3) 6 4_446
O3 Ta Ga3 87.3(3) 5 4_446
O3 Ta Ga3 160.1(3) 4 4_446
Ga3 Ta Ga3 106.21(6) 4_445 4_446
O3 Ta Ga3 54.3(3) 2 1_656
O3 Ta Ga3 97.9(3) 3 1_656
O3 Ta Ga3 160.1(3) . 1_656
O3 Ta Ga3 87.3(3) 6 1_656
O3 Ta Ga3 31.7(3) 5 1_656
O3 Ta Ga3 113.8(3) 4 1_656
Ga3 Ta Ga3 145.06(2) 4_445 1_656
Ga3 Ta Ga3 62.66(4) 4_446 1_656
O3 Ta Ga3 113.8(3) 2 1_655
O3 Ta Ga3 31.7(3) 3 1_655
O3 Ta Ga3 87.3(3) . 1_655
O3 Ta Ga3 160.1(3) 6 1_655
O3 Ta Ga3 97.9(3) 5 1_655
O3 Ta Ga3 54.3(3) 4 1_655
Ga3 Ta Ga3 62.66(4) 4_445 1_655
Ga3 Ta Ga3 145.06(2) 4_446 1_655
Ga3 Ta Ga3 106.21(6) 1_656 1_655
O3 Ta Ga3 87.3(3) 2 2_565
O3 Ta Ga3 160.1(3) 3 2_565
O3 Ta Ga3 113.8(3) . 2_565
O3 Ta Ga3 31.7(3) 6 2_565
O3 Ta Ga3 54.3(3) 5 2_565
O3 Ta Ga3 97.9(3) 4 2_565
Ga3 Ta Ga3 145.06(2) 4_445 2_565
Ga3 Ta Ga3 62.66(4) 4_446 2_565
Ga3 Ta Ga3 62.66(4) 1_656 2_565
Ga3 Ta Ga3 145.06(2) 1_655 2_565
O3 Ta Ga3 160.1(3) 2 2_564
O3 Ta Ga3 87.3(3) 3 2_564
O3 Ta Ga3 54.3(3) . 2_564
O3 Ta Ga3 97.9(3) 6 2_564
O3 Ta Ga3 113.8(3) 5 2_564
O3 Ta Ga3 31.7(3) 4 2_564
Ga3 Ta Ga3 62.66(4) 4_445 2_564
Ga3 Ta Ga3 145.06(2) 4_446 2_564
Ga3 Ta Ga3 145.06(2) 1_656 2_564
Ga3 Ta Ga3 62.66(4) 1_655 2_564
Ga3 Ta Ga3 106.20(6) 2_565 2_564
O2 Ga2 O2 98.6(6) 4_445 3_455
O2 Ga2 O2 98.6(6) 4_445 .
O2 Ga2 O2 98.6(6) 3_455 .
O2 Ga2 O1 118.9(5) 4_445 2_456
O2 Ga2 O1 118.9(5) 3_455 2_456
O2 Ga2 O1 118.9(5) . 2_456
O2 Ga2 La 43.0(4) 4_445 2_455
O2 Ga2 La 55.8(4) 3_455 2_455
O2 Ga2 La 105.9(5) . 2_455
O1 Ga2 La 134.75(4) 2_456 2_455
O2 Ga2 La 55.8(4) 4_445 4_445
O2 Ga2 La 105.9(5) 3_455 4_445
O2 Ga2 La 43.0(4) . 4_445
O1 Ga2 La 134.74(4) 2_456 4_445
La Ga2 La 75.92(6) 2_455 4_445
O2 Ga2 La 105.9(5) 4_445 .
O2 Ga2 La 43.0(4) 3_455 .
O2 Ga2 La 55.8(4) . .
O1 Ga2 La 134.74(4) 2_456 .
La Ga2 La 75.92(6) 2_455 .
La Ga2 La 75.92(6) 4_445 .
O2 Ga2 La 98.6(5) 4_445 4_446
O2 Ga2 La 159.5(5) 3_455 4_446
O2 Ga2 La 89.5(4) . 4_446
O1 Ga2 La 41.89(4) 2_456 4_446
La Ga2 La 139.567(7) 2_455 4_446
La Ga2 La 92.856(7) 4_445 4_446
La Ga2 La 139.566(7) . 4_446
O2 Ga2 La 89.5(4) 4_445 2_456
O2 Ga2 La 98.6(5) 3_455 2_456
O2 Ga2 La 159.5(5) . 2_456
O1 Ga2 La 41.89(4) 2_456 2_456
La Ga2 La 92.855(7) 2_455 2_456
La Ga2 La 139.567(7) 4_445 2_456
La Ga2 La 139.566(7) . 2_456
La Ga2 La 70.65(6) 4_446 2_456
O2 Ga2 La 159.5(5) 4_445 1_556
O2 Ga2 La 89.5(4) 3_455 1_556
O2 Ga2 La 98.6(5) . 1_556
O1 Ga2 La 41.89(4) 2_456 1_556
La Ga2 La 139.566(7) 2_455 1_556
La Ga2 La 139.566(7) 4_445 1_556
La Ga2 La 92.855(7) . 1_556
La Ga2 La 70.65(6) 4_446 1_556
La Ga2 La 70.65(6) 2_456 1_556
O3 Ga3 O3 133.5(6) 3_455 5_454
O3 Ga3 O2 108.4(5) 3_455 3_454
O3 Ga3 O2 100.1(6) 5_454 3_454
O3 Ga3 O2 100.1(6) 3_455 5_455
O3 Ga3 O2 108.4(5) 5_454 5_455
O2 Ga3 O2 103.0(7) 3_454 5_455
O3 Ga3 Ta 109.8(3) 3_455 1_454
O3 Ga3 Ta 35.7(3) 5_454 1_454
O2 Ga3 Ta 86.4(4) 3_454 1_454
O2 Ga3 Ta 144.1(4) 5_455 1_454
O3 Ga3 Ta 35.7(3) 3_455 1_455
O3 Ga3 Ta 109.8(3) 5_454 1_455
O2 Ga3 Ta 144.1(4) 3_454 1_455
O2 Ga3 Ta 86.4(4) 5_455 1_455
Ta Ga3 Ta 106.20(6) 1_454 1_455
Ga2 O1 La 109.5(5) 2_566 .
Ga2 O1 La 109.5(5) 2_566 4_455
La O1 La 109.5(5) . 4_455
Ga2 O1 La 109.5(5) 2_566 2_565
La O1 La 109.5(5) . 2_565
La O1 La 109.5(5) 4_455 2_565
Ga2 O2 Ga3 117.2(9) . 4_446
Ga2 O2 La 105.7(5) . 4_445
Ga3 O2 La 119.5(5) 4_446 4_445
Ga2 O2 La 91.6(4) . .
Ga3 O2 La 112.6(5) 4_446 .
La O2 La 106.2(5) 4_445 .
Ga3 O3 Ta 112.5(4) 4_445 .
Ga3 O3 Ga1 112.5(4) 4_445 .
Ta O3 Ga1 0.0 . .
Ga3 O3 La 138.9(5) 4_445 .
Ta O3 La 104.0(5) . .
Ga1 O3 La 104.0(5) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
La O3 2.392(9) 6
La O3 2.392(9) .
La O2 2.398(14) 3_455
La O2 2.398(14) 5_455
La O1 2.551(7) 2_455
La O1 2.551(7) .
La O2 2.800(11) .
La O2 2.800(11) 6
La Ga2 3.385(2) .
La Ga2 3.385(2) 2_565
La Ga1 3.4710(9) .
La Ta 3.4710(9) .
Ga1 O3 2.002(10) 2
Ga1 O3 2.002(10) 3
Ga1 O3 2.002(10) .
Ga1 O3 2.002(10) 6
Ga1 O3 2.002(10) 5
Ga1 O3 2.002(10) 4
Ga1 La 3.4710(9) 2
Ga1 La 3.4710(9) 4
Ta O3 2.002(10) 2
Ta O3 2.002(10) 3
Ta O3 2.002(10) .
Ta O3 2.002(10) 6
Ta O3 2.002(10) 5
Ta O3 2.002(10) 4
Ta Ga3 3.1662(11) 4_445
Ta Ga3 3.1662(11) 4_446
Ta Ga3 3.1662(11) 1_656
Ta Ga3 3.1662(11) 1_655
Ta Ga3 3.1662(11) 2_565
Ta Ga3 3.1662(11) 2_564
Ga2 O2 1.826(12) 4_445
Ga2 O2 1.826(12) 3_455
Ga2 O2 1.826(12) .
Ga2 O1 1.83(2) 2_456
Ga2 La 3.385(2) 2_455
Ga2 La 3.385(2) 4_445
Ga2 La 3.601(3) 4_446
Ga2 La 3.601(3) 2_456
Ga2 La 3.601(3) 1_556
Ga3 O3 1.803(10) 3_455
Ga3 O3 1.803(10) 5_454
Ga3 O2 1.890(13) 3_454
Ga3 O2 1.890(13) 5_455
Ga3 Ta 3.1662(11) 1_454
Ga3 Ta 3.1662(11) 1_455
O1 Ga2 1.83(2) 2_566
O1 La 2.551(7) 4_455
O1 La 2.551(7) 2_565
O2 Ga3 1.890(13) 4_446
O2 La 2.398(14) 4_445
O3 Ga3 1.803(10) 4_445
